CATALYTIC HYDROGENOLYSIS OF GLYCEROL
For the degree of
DOCTOR OF PHILOSOPHY in
INORGANIC AND PHYSICAL CHEMISTRY DIVISION
INDIAN INSTITUTE OF CHEMICAL TECHNOLOGY
HYDERABAD-500 607, INDIA
CATALYTIC HYDROGENOLYSIS OF GLYCEROL
The usage of bio-fuels for transportation, in place of
petroleum-derived fuels, will increase world over in the coming decades. Among the
bio-fuels contemplated for use, bio-ethanol and biodiesel are the important
ones. Particularly, the demand for biodiesel is expected to increase in the
Glycerol is a by-product of biodiesel industry. Approximately 10 wt %
of glycerol is formed in the manufacture of biodiesel by transesterification of
seed oils with methanol. It is identified as a potentially important bio-refinery
feedstock. Glycerol has a great number of applications and it has been used
in pharmaceuticals, cosmetics, soaps, toothpastes, candies, cakes and as a
wetting agent in tobacco. However, there has been glut in the global market
due to increased production of biodiesel. It is a big challenge to use this
low-grade glycerol obtained from biodiesel production as it cannot be used for
food and cosmetic uses. Today, there is a need to develop process
technologies for the value-addition of glycerol to improve the economics of
biodiesel production. New chemistry of glycerol is emerging increasing the
role of glycerol in future bio-refineries. Further, the derivatives of glycerol
also are finding use in sectors as diverse as fuels, chemicals, automotive,
pharmaceutical, detergent, and building materials.
Glycerol is a highly functionalized molecule; a variety of value-added
different reactions via a different reaction routes, such as oxidation,
hydrogenolysis, dehydration, pyrolysis, steam reforming, etherification,
esterification, oligomerisation, and polymerization. Here again the
conversion by green catalytic processes is a challenging area of research. It
is required to develop highly active heterogeneous catalysts to produce the
desired chemical from crude glycerol.
1,2-propanediol (1,2-PDO) or propylene glycerol is a three-carbon diol
with a stereogenic center at the central carbon atom. It is an important
medium-value commodity chemical with a 4% annual growth in the global
market. It is used for making polyester resins, liquid detergents,
pharmaceuticals, cosmetics, tobacco humectants, flavor and fragrance
agents, personal care items, paints, animal feed, antifreeze compound, etc.
There has been a rapid expansion of the market for 1,2-PDO as antifreeze
and de-icing agent because of the growing concern over the toxicity of
ethylene glycol based products to humans and animals. Presently, the
propylene glycol market is under severe pressure due to increase in oil and
natural gas costs as these form the basic raw materials. Glycerol can be
converted to 1,2-PDO using heterogeneous, homogeneous or biocatalysts.
Among all these, heterogeneous catalytic conversion of glycerol is
economically and environmentally attractive.
The work presented in this thesis is aimed at developing an active and
selective heterogeneous catalyst for the hydrogenolysis of glycerol to
combination with solid acids (taken as co-catalysts catalysts) has been
tested and the role of solid acid is described. An attempt has been made to
prepare hybrid materials with both metal and acid functions in the same
catalyst. A detailed study has been made on the application of non-noble
metals, such as Cu and Ni, for the hydrogenolysis. Finally, the non noble
metal catalysts have been promoted with Cr to improve the conversion and
1,2-PDO selectivity. The catalysts have been characterized thoroughly to
elucidate the structure-activity relationship.
Aims and Objectives:
1. The principal aim of this thesis is to develop a highly active
for selective hydrogenolysis of glycerol selecting both noble and
2. Studying the influence of solid acids as co-catalysts on glycerol
hydrogenolysis to 1,2-PDO over Ru/C to identify the importance of acidity
on the catalytic functionality.
3. Identification of the suitability of preparing a hybrid catalyst by
depositing Ru on the acid support, instead of taking the two components
4. Studying of glycerol hydrogenolysis functionality of Cu and Ni based
5. Elucidation of the role of Cr promoter on Cu-Zn catalysts for glycerol
6. Detailed characterization of the catalysts and correlating their
properties with activity, and
7. Understanding the reaction mechanism to achieve the specific
Scope of the work:
Catalytic hydrogenolysis of glycerol was studied over supported noble
metal and mixed oxide catalysts. Active carbon supported Ru, Pt, Rh and Pd
catalysts were studied for glycerol hydrogenolysis and Ru/C was identified as
the best catalyst. The influence of inclusion of solid acid catalysts, like ion
exchange resins, on the activity of Ru/C was identified. The relationship
between acidity of solid acid and conversion was brought out. The second
generation hybrid catalysts were prepared by supporting Ru on various solid
acid materials (ZrO2, Nb2O5 and TiO2) and their efficiency in catalyzing the
hydrogenolysis is ascertained. Non-noble metal based Cu-Zn, Cu-Mg and
Ni-Zn catalysts were prepared by co-precipitation method and evaluated them
for the selective hydrogenolysis. In order to increase the activity of Cu-Zn
catalysts, Cr was added as a structural promoter and the improvements in
the functionality of the catalyst were delineated. The effect of variation in
catalysts were characterized thoroughly to establish structure - activity
Organization of the thesis:
It gives a brief introduction on the commercial importance of glycerol
and 1,2-PDO. The importance of value addition of glycerol is touched upon.
The various methods available for value-addition of glycerol are discussed.
The advantages of glycerol hydrogenolysis over the other reactions are
addressed. A detailed account of the need for the development of
heterogeneous catalysts for selective glycerol hydrogenolysis is given. The
aim, objectives and scope of the work in carrying out the hydrogenolysis of
glycerol over supported Ru catalysts and non-noble metal (Cu, Ni) catalysts,
prepared by different methods, is discussed.
Chapter 2: Literature review
The various catalysts developed and studied for glycerol
hydrogenolysis are discussed. The related literature on noble and non -noble
metal catalysts is given in this chapter. The variation in hydrogenolysis
activity between noble and non -noble metal catalysts is discussed briefly.
The reaction mechanisms proposed over various catalytic systems are also
General procedures for catalyst preparation like impregnation,
deposition-precipitation and precipitation along with the methodologies
followed in the present work are presented in this chapter. The basic
concepts and the experimental procedures of catalyst characterization
techniques are described. The methodologies followed in the present work to
evaluate the catalysts during glycerol hydrogenolysis are also discussed in
detail. The preparation of supported Ru catalysts by impregnation and
deposition-precipitation methods using RuCl3.XH2O as metal precursor and
the mixed oxide catalysts such as Cu-Zn, Cu-Mg, Ni-Zn and Cu-Cr-Zn with
varying Cu/M, Ni/Zn mole ratio prepared by co-precipitation method are
The principles and the actual conditions used in the characterization of
catalysts are narrated. N2 gas adsorption for BET surface area, XRD, TPR, TEM,
TPD of NH3 and XPS techniques are described in detail.
Results and Discussion:
Chapters-4, 5 and 6 represent the results and discussion part of the thesis.
They essentially deal with results obtained during the activity studies on
Further, the characterization results of all these catalysts obtained by
various techniques are correlated with the activity.
Chapter 4: Glycerol hydrogenolysis activity on supported
This chapter consists of three sections. The individual sections
describe the results obtained during glycerol hydrogenolysis over Ru based
catalysts. In each section, the results obtained on studies aimed at
identification of the effect of different reaction parameters are highlighted.
The activity results are correlated with the physico-chemical properties of
Section 4.1: Glycerol hydrogenolysis activity on carbon
supported noble metal catalysts with Amberlyst 15 as
In the present study, selective hydrogenolysis of glycerol into 1,2-PDO
studied over active carbon supported noble metal catalysts such as Pt/C, Pd/
C, Rh/C and Ru/C as metal function catalysts is reported. Ru/C catalyst has
shown the highest glycerol conversion than Pt/C, Pd/C and Rh/C catalysts.
However, the main product is derived from C-C bond cleavage in the
hydrogenolysis reaction in the case of Ru/C leading to the degradation
product ethylene glycol. The glycerol hydrogenolysis activity over M/C in
combination with Amberlyst 15 catalysts (M = Pt, Rh, Pd, and Ru) is then
taken up. Here, Amberlyst 15 is used as a solid acid catalyst. The addition of
Amberlyst to supported noble metal catalyst showed higher hydrogenolysis
activity than the supported metal catalysts when used alone. The
hydrogenolysis activity of glycerol increased from 5.2 to 11.2 % in case of
Ru/C when used in combination with Amberlyst. Hydrogenolysis of glycerol
(SHR) is possible when metal supported catalysts alone are used. The
addition of solid acid to metal catalysts enhances the conversion and
selectivity of the reaction because, hydrogenolysis proceeds through a
two-step mechanism. Dehydration of glycerol to acetol takes place in first two-step
over solid acid catalyst followed by hydrogenation in next step over metal
site. According to the results obtained in this part of the thesis, the glycerol
conversion into 1,2-PDO proceeded by combination of dehydration over
Amberlyst catalyst and subsequent hydrogenation over metal catalysts.
Thus, it is observed that the solid acid catalyst plays a major role in glycerol
hydrogenolysis. Acetol is a reaction intermediate as it was identified in high
concentrations by gas chromatography. Therefore, high glycerol conversions
and high selectivity to propylene glycol could be achieved when Amberlyst
was used as solid acid catalyst.
The relative importance of acid or metal catalyst in the hydrogenolysis
of glycerol was studied by varying the individual catalyst weights. A
synergetic effect between acid catalyst and metal catalyst was observed.
The catalytic system gave better selectivity with good conversion when the
weight ratio of Amberlyst to Ru/C was 2. Increasing the catalyst amounts by
keeping their ratio same increased the overall glycerol conversion
remarkably. The effect of reaction temperature on the stability of Amberlyst
catalyst was studied. The decomposition of Amberlyst at high temperatures
Section 4.2: Effect of the nature of solid acid on the
glycerol hydrogenolysis activity of Ru/C catalyst
Selective hydrogenolysis reaction was studied over Ru/C catalyst with
several solid acids like zeolites (ZSM-5, Hb, Y-Zeolite), mesoporous SiO2
(SBA-15, MCM-41), metal oxides (Nb2O5, TiO2, ZrO2) and heteropoly acids
(TPA/CsZrO2, CsTPA, CsTPA/ZrO2, TPA/ZrO2) as co-catalysts. The glycerol
conversion and 1,2-PDO selectivity varied with the nature of solid acid under
the same reaction conditions. It was proved that the acidity of the catalyst
also influences its glycerol hydrogenolysis activity. In order to understand
the relation between glycerol conversion and acid strength of the co-catalyst,
temperature programmed desorption of ammonia (TPDA) was carried out
over solid acids. TPDA results suggested that the total acidity of the catalyst
plays a major role in the overall glycerol conversion. It also suggested that
moderate acid sites are sufficient to get reasonable glycerol conversion.
Section 4.3: Glycerol hydrogenolysis over solid acid
supported Ruthenium catalysts
In the previous section describes the results obtained taking different
solid acids as co-catalysts in combination with Ru/C for glycerol
systems leads to non-concurrent results . Therefore, a single hybrid
catalyst is thought to overcome this disadvantage. Ru was supported on
various solid acids to make a single catalytic system for this reaction.
Different bi-functional catalysts were prepared and evaluated for the
hydrogenolysis activity. It is observed that the nature of support material as
well as its method of preparation influences the catalytic performance in the
presence of ruthenium metal.
Chapter 5: Glycerol hydrogenolysis activity on non-noble
metal mixed oxide catalysts
This chapter explains the glycerol hydrogenolysis over non-noble metal
catalysts. The hydrogenolysis activity of Cu-Zn, Cu-Mg and Ni-Zn catalysts
are discussed in detail. The effect of different reaction parameters is also
presented. High activity of the catalysts is explained with the help of
Section 5.1: Selective hydrogenolysis of glycerol to
1,2-propanediol over Cu-Zn catalysts
Cu-Zn catalyst can be used for selective hydrogenolysis of glycerol due
to the acidic nature of ZnO and hydrogenation ability of Cu in the Cu-ZnO
catalyst. These catalysts were prepared and evaluated for selective
hydrogenolysis of glycerol to propylene glycol. The results suggested that
optimum conversion was recorded for the catalyst with Cu to Zn ratio of 1. It
is found that the hydrogenolysis activity mainly depends on Cu metal area
and its dispersion.
Section 5.2: Selective hydrogenolysis of glycerol to
1,2-propanediol over Cu-Mg catalysts
As discussed in previous section, a selectivity to 1,2-PDO of more
than 90 % was achieved over Cu-Zn catalysts. However, the hydrogenolysis
activity of catalyst was low. Therefore, the hydrogenolysis was performed
on Cu-Mg catalysts prepared via co-precipitation and by varying Cu loading.
Cu-Mg catalyst was found to be more active than Cu-Zn catalyst. The results
have been explained based on the reaction mechanisms proposed in the
Section 5.3: Selective hydrogenolysis of glycerol to
1,2-propanediol over Ni-Zn catalysts
Muhler et al. have reported the growth of copper particles in a
Cu/ZnO methanol catalyst with increasing time on stream. A similar
behavior was also observed in the case of hydrogenolysis carried out on Cu
based catalysts. As ZnO stabilizes the metal species on its surface, Ni-Zn
catalysts were studied for the hydrogenolysis activity. Ni-Zn catalyst showed
greater performance in the liquid phase hydrogenolysis reaction.
The Effect of Ni/Zn mole ratio on glycerol hydrogenolysis was studied.
ratio of 2. It is found that the catalyst having high metal surface offers high
Chapter 6: Glycerol hydrogenolysis activity on Cr
promoted Cu based catalysts
Cu-Zn catalysts showed poor glycerol hydrogenolysis activity under
mild reaction conditions. However, the selectivity towards propylene glycol
was appreciable. Harsh reaction conditions or long reaction runs could get
higher glycerol conversion over Cu-Zn catalysts, but the selectivity
decreases with increase in glycerol conversion at high reaction temperature
and hydrogen pressures. Hence, there was a need to increase the activity of
Cu-Zn catalysts towards obtaining better glycerol conversion, still retaining
high propylene glycol selectivity under mild reaction conditions. Therefore,
Cr promoted Cu-Zn catalysts were prepared and evaluated for glycerol
hydrogenolysis. With the addition of Cr the conversion increased by about 7
times in comparison with bulk copper oxide and the selectivity of 1,2PDO
was obviously improved to 95%. The present result was better than those
reported in the literature. The order of conversion of glycerol for copper
oxide catalysts was as follows: CuCrZn>CuZn>CuCr>CuO.
Chapter 7: Overall conclusions
This chapter describes the important conclusions drawn from the work
Glycerol hydrogenolysis activity on supported Ru catalysts
Ru/C gives the highest glycerol conversion among Pt/C, Pd/C and Rh/C
catalysts. The main product (1,2-PDO) is derived from C-C bond cleave in the
hydrogenolysis leading to the formation of degradation product, ethylene
glycol. The addition of ion exchange resin to metal catalyst increases the
glycerol conversion as well as selectivity to 1,2-PDO. The promoting effect of
Amberlyst is low for Pt/C, Rh/C and Pd/C compared to Ru/C. The addition of
solid acid to metal catalysts enhances the conversion and selectivity of the
reaction because, the hydrogenolysis proceeds through a two-step
The activity of the catalyst in glycerol hydrogenolysis depends up on
the amount of the acidity of solid acid taken as co-catalyst. A synergistic
effect can be observed between solid acid and Ru/C catalyst towards glycerol
conversion and selectivity to 1,2-PDO.
In the case of the hybrid catalyst, (Ru supported metal oxides), the
method of catalyst preparation can influence the conversion and selectivity
during glycerol hydrogenolysis. The catalyst prepared by DP method shows
higher conversion than the IM catalysts. The presence of residual chloride
has detrimental effect on glycerol hydrogenolysis for supported Ru catalysts.
Glycerol hydrogenolysis activity on non-noble metal mixed
Selective formation of 1,2-PDO can be achieved at low hydrogen
important effect on glycerol conversion. The presence of small Cu and ZnO
particles are required for better activity in glycerol hydrogenolysis.
Replacing of ZnO with MgO in Cu based catalysts alters the reaction
mechanism of hydrogenolysis reaction. Cu-Mg catalysts show better activity
than the Cu-Zn catalyst. Even though Cu based catalysts show better
activity compared to supported Ru catalysts, their reusability is very poor.
The deactivation rate of the copper based catalyst is high due to
agglomeration of the metal crystallites.
In the case of Ni-Zn, the activity of the catalyst depends on the Ni/Zn
ratio. High glycerol conversion can be achieved over Ni/Zn catalyst mole
ratio of 2. The glycerol conversion is favored on small particle sizes of Ni and
ZnO. The presence of well dispersed Ni particles on ZnO is essential to get
high activity in glycerol hydrogenolysis. Ni-Zn catalyst shows the consistent
activity upon reuse.
Glycerol hydrogenolysis activity on Cr promoted Cu based
Ternary Cu-Cr-Zn oxide shows high glycerol conversion than binary Cu/
Cr, Cu/Zn and single CuO oxide catalysts. Acidity and metal surface area of
the catalysts increases by the addition of Cr and Zn to CuO. Even very low
amounts of Cr in Cu-Zn catalyst affects the acidity and metal surface of the
catalysts leading to high glycerol conversion. Enhancement in the acidity and
Systematic study on the catalytic hydrogenolysis of glycerol over
supported Ru catalysts and mixed metal oxide catalysts.
Synthesis of highly active and selective solid acid catalysts for glycerol
Replacement of ion exchange resins with thermally stable solid acid
Elucidation of the influence of solid acid in combination with carbon
supported Ru catalysts
Development of a single hybrid catalyst in place of two catalyst systems.
Development of inexpensive non-noble metal oxide based catalyst in
place of noble metal catalysts.
Synthesis of high active, selective to 1,2-PDO and recyclable Ni-Zn
catalysts for glycerol hydrogenolysis.
Development of high active Cu based catalysts by the addition of Cr as
List of Publications
1. Surface and structural properties of titania supported Ru catalysts for hydrogenolys
M. Balaraju, V. Rekha, B.L.A. Prabhavathi Devi, R. B. N. Prasad, P.S. Sai Prasad, N.
Lingaiah; Applied Catalysis A: General 384 (2010) 107-114.
2. Selective esterification of glycerol to bioadditives over heteropoly tungstate
supported on Cs containing zirconia catalysts
K. Jagadeeswaraiah, M. Balaraju, P.S. Sai Prasad, N. Lingaiah; Applied Catalysis
A: General 386 (2010) 166–170.
3. Acetylation of glycerol to synthesize bioadditives over niobic acid supported
tungstophosphoric acid catalysts
M. Balaraju, P. Nikhitha, K. Jagadeeswaraiah, K. Srilatha, P.S. Sai Prasad, N.
Lingaiah*; Fuel Processing Technology, 91 (2010) 249-253.
4. Influence of solid acids as co-catalysts on glycerol hydrogenolysis to propylene
glycol over Ru/C catalysts
M. Balaraju, V. Rekha, P.S. Sai Prasad, B.L.A. Prabhavathi Devi, R.B.N. Prasad,
N. Lingaiah; Applied Catalysis A: General 354 (2009) 82–87
5. Selective hydrogenolysis of glycerol to 1, 2 propanediol over Cu–ZnO catalysts
M. Balaraju, V. Rekha, P. S. Sai Prasad, R. B. N. Prasad N. Lingaiah, Catalysis
Letters 126 (2008)119–124.
6. Synthesis and characterization of zirconia supported vanadium incorporated
K. Mohan Reddy, M. Balaraju, P. S. Sai Prasad, I. Suryanarayana, N. Lingaiah,
Catalysis Letters 119 (2007)304–310.
7. Selective oxidation of allylic alcohols catalyzed by silver exchanged molybdovanado phosphoric acid catalyst in the presence of molecular oxygen
P. Nagaraju, M. Balaraju, K. Mohan Reddy, P.S. Sai Prasad, N. Lingaiah , Catalysis
Communications 9 (2008) 1389–1393.
8. Studies on vanadium-doped iron phosphate catalysts for the ammoxidation of
P. Nagaraju, N. Lingaiah, M. Balaraju, P. S. Sai Prasad , Applied Catalysis A:
General 339 (2008) 99–107.
1. Selective Hydrogenolysis of Glycerol to 1,2-Propanediol over Ni-Zn Catalysts
M. Balaraju, K. Jagadeeswaraiah, P.S. Sai Prasad, N. Lingaiah
(Communicated to CHEMCATCHEM)
2. Cr promoted Cu based catalyst for Selective Hydrogenolysis of Glycerol to Propylene
M. Balaraju, P.S. Sai Prasad, N. Lingaiah, A. K. Dalai (to be
List of Patents
1. Catalytic process for the preparation of 1,2-propanediol by selective hydrogenolysis of glycerol. (Under process)
Papers presented at symposiums
1. Hydrogenolysis of glycerol over Ru based bifunctional catalysts (Oral presentation)
M. Balaraju, N.Lingaiah, P. S. Sai Prasad
19th National Symposium on Catalysis, NCL, Pune India, January 2009.
2. Surface and structural properties of supported Ru catalysts for hydrogenolysis of
Glycerol (Poster presentation)
M. Balaraju, V. Rekha, B.L.A. Prabhavathi Devi ,R. B. N. Prasad, P.S. Sai Prasad,
12th CRSI National Symposium in Chemistry, IICT, Hyderabad, January,
3. Synthesis of glycerol carbonate from glycerol and dimethyl carbonate over
Mg/Al/Zr catalyst (Poster presentation)
M. Malyaadri, K.Jagadeeswaraiah, M. Balaraju, P. S. Sai Prasad, N. Lingaiah
20th National Symposium on Catalysis, IIT, Chennai, India, December,
4. Glycerol into value added chemicals (Poster presentation)
M. Balaraju, K. Jagadeeswaraiah, M. Malyaadri, P.S. Sai Prasad, N. Lingaiah
International Conference on Recent trends in Renewable Energy Resources,